Catalysis Today 30 (1996) 59-65
The performance and structure of rare earth oxides modified by strontium fluoride for methane oxidative coupling Ruiqiang Long, Yaping Huang, Weizheng Weng, Huilin Wan *, Khirui Tsai Department
ofChemistryand State Key Laboratory forPhysical Chemistry of the Solid Surjke,
Xiamen Unil;ersity, Xiamen, 361005, China
Abstract Strontium fluoride promoted rare earth (La, Nd, Sm, Eu, Gd, Dy, and Y) oxides were more selective than the corresponding unpromoted rare earth oxides for the methane oxidative coupling to ethane and ethene. The XRD results indicated that the partial anionic or cationic exchanges and interaction between the oxide and fluoride phases took place in most of the catalysts studied in this paper, leading to the formation of new oxyfluoride phases. The possible formation of anionic vacancies in the lattice as the result of ionic exchange and interaction between the phases will be favorable to the activation of molecular oxygen and the improvement of catalytic performance. Keywords: Methane oxidative
fluoride; Ionic exchange; Anionic vacancy
1. Introduction Methane oxidative coupling (MOC) to Cz+ hydrocarbons has been a much investigated area in recent decade. A large number of catalysts has been found to be active and selective for the formation of ethane and ethene. Among these catalysts, the rare earth oxides (REO), especially Sm,O, and La203, have been extensively studied as MOC catalysts due to their high catalytic activities and selectivities as well as satisfactory thermal stabilities [l-4]. In order to further improve the catalytic performance of REO catalysts for MOC reaction, some promoters, usually alkali-metal or alkaline earth-metal
0920-5861/96/$32.00 0 1996 Elsevier Science B.V. All rights reserved SSDI 0920-5861(95)00328-2
oxides, have been added to the REO catalyst systems [5,6]. However, these alkali-metal or alkaline earth-metal oxides doped catalysts usually exhibit strongly basic property, and are easily poisoned by the CO, generated during the reaction, so that a higher reaction temperature is required to maintain an adequate level of activity. Besides the promotional effect of metal oxides mentioned above, the benefits of addition of chlorinated compounds to the MOC reaction have also been reported by many research groups [7-lo]. Recently, Lunsford et al. [9,10] reported a Cl- promoted Li+--MgO catalyst which showed good catalytic performance for both MOC and ODE (oxidative dehydrogenation of ethane). In contrast to the unpromoted Li+--MgO system, alkane conversions over the Lif-MgO-Clcatalysts with a Cl/Li
R. Long et al. /Catalysis
Today 30 (1996) 59-65
ratio of 0.9 were almost unaffected by CO,, since the presence of Cl- ions at an appropriate level modified the catalyst so that it no longer functioned as a strongly basic oxide catalyst and would therefore not be easily poisoned by CO,. In addition to chlorinated compounds, We have recently found that metal fluorides also showed significant promotional effects on the oxide catalysts for the MOC and oxidative dehydrogenation of light alkanes (C,H, and C,H,) reactions [ 1l- 131. The beneficial effects resulting from addition of fluorides to oxides include (i) possible formation of lattice defects, such as anionic vacancies, which are requisite for the adsorption and activation of 0, over the catalysts with stable cationic valencies, (ii) modification of the basicity of metal oxides, and (iii) isolation of the surface active oxygen species. In this work, the catalytic property of a series of SrF, promoted Ln,O, catalysts with Ln = La, Nd, Sm, Gd, Eu, Dy and Y will be reported. Attention will be focused on the correlations between catalytic properties and the bulk composition and structure of the catalysts.
Table I Catalytic
Catalyst (mole ratio)
Blank experiment SrF, La203
SrF,/La,O, SrF,/La,O, NdzO, SrF,/Nd,O,
(1:4) (1:l) (1:l)
SrF2/Eu,03 Gd,Os SrF,/Gd,O,
of the SrF,/Ln,O,
750 750 750 700 700 750 750 750 800 800 750 750 750 750 750 750 750 750
The SrF, promoted catalysts were prepared by grinding different mole ratios of rare earth oxides (La,O,, Nd,O,, Sm,O,, Gd,O,, Eu,O,, Dy,O, and Y203, purity > 99.5%) with SrF, into fine powder. The mixture was then mixed with certain amount of deionized water to form a paste, followed successively by drying at 120°C for 4 h and calcining at 900°C (850°C for SrF,/Sm,O,) for 6 h. The resulting solid was crushed and sieved to 40-60 mesh particles. The pure rare earth oxides and SrF, used for the catalytic performance evaluation were also treated with the similar procedures as described above. Unless indicated elsewhere, the reagents used in the preparation were of analytical grade. The catalytic reactions were carried out in a fixed bed quartz reactor (5.0 mm inside diameter) under the conditions of GHSV = 20000 h- ’ and CH,/O, = 3 (mole ratio). Methane (99.99%) and oxygen (99.5%) were used without further purification. In each experimental run, 0.20 ml of catalyst was used, and the
for the oxidative coupling
no activity 0.7 2.4 29.8 100 29.4 100 34.2 98.1 35.6 99.2 27.2 99.1 34.3 98.9 26.3 99.2 34.0 99.5 26.3 98.4 33.1 99.0 29.5 99.7 34.4 99.5 31.3 99.5 32.6 96.3 27.2 98.3 33.6 94.4
0.0 10.2 10.5 6.4 10.6 7.2 4.0 8.9 3.9 13.8 6.7 17.5 5.9 12.4 8.5 16.9 8.3
46.0 52.0 52.3 36.3 34.3 53.5 38.9 52.3 40.3 53.1 40.4 49.0 39.5 45.0 40.0 50.2 35.1
0.0 20.0 21.5 36.1 31.4 20.1 33.1 21.6 33.1 21.8 31.9 20.1 32.0 25.0 32.0 20.1 34.1
54.0 15.8 15.7 21.2 23.7 19.2 24.0 17.2 22.7 11.3 21.0 13.4 22.6 17.6 19.5 12.8 22.5
54.0 35.8 37.2 57.3 55.1 39.3 57.1 38.8 55.8 33.1 52.9 33.5 54.6 42.6 51.5 32.9 56.6
= 3:1, no inert gas for dilution, GHSV = 20000 h-t.
The data were obtained after 30 min on stream.
0.4 10.7 10.9 19.6 19.6 10.7 19.6 10.2 19.0 8.7 17.5 9.9 18.8 13.3 16.8 9.0 19.0
R. Long et al. / Catalysis Today 30 (1996) 59-65
gaseous effluent was analyzed at room temperature by an on-line Shang Fen 102GD gas-chromatograph equipped with thermal conductivity detector, with 5A molecular sieve column for 0, and CO, and GDX 502 column for CH,, C,H,, C,H, and CO,. The conversion of methane (C methane)and selectivities of the products (SJ were calculated from the equations: c methane = ( ZAi X Fi)/[ 2 ( Ai X F):)+ Amethane x &&lane] and Si = ( Ai X Fi>/l?( Ai X F;.), respectively, where A = peak area of carbon-containing species and F = correction factor of response and carbon number. The XRD measurements were carried out at room temperature on a Rigaku Rotaflex D/Max-C system with Cu K a( h = 1S406 A> radiation. The samples were loaded on a sample holder with depth of 1 mm. XRD patterns were recorded in the range of 2 8 = 20-70”.
3. Results and discussion 3.1. Catalytic per$ormance evaluation The catalytic performances of a series of SrF, promoted rare earth sesquioxide catalysts with different SrF,/Ln,O, mole ratios were evaluated and the results were summarized in Table 1. The blank reactor was found to have no activity for the reaction between CH, and 0, at
For pure rare earth oxides, such as La,O,, Nd,O,, Sm,O,, Eu,O, Gd,O, and Y203 catalysts, 26-31% of CH, conversions with 30-43% of C, selectivities were obtained. When a certain amount of SrF,, which had almost no activity for MOC reaction, was added to the oxide catalysts, CO, (CO + CO,) selectivities decreased significantly, while C 2 selectivities and yields were apparently improved under the same conditions, indicating that the addition of SrF, plays a significant promoting role for the MOC reaction with these REO as catalysts. Maximum C, yield of 19.6% was observed over SrF,/La,O, (1:4) and SrF,/Nd,O, (1: 1) catalyst, respectively, which was about 9% higher than those over pure La,O, and Nd,O, under the same conditions. Comparatively, the promotional effect of SrF, on Dy,O, was rather unpronounced, and similar results were also observed on the SrF, modified Ho,O,, Er,O,, Tm,O, and Yb,O, catalysts. This phenomenon may have resulted from the interaction between SrF, and Ln,O, of which Ln = Dy, Ho, Et-, Tm and Yb were relatively weak as compared with the other SrF, modified rare earth sesquioxide catalysts studied in this paper. It has been known that the conductivities of rare earth sesquioxides decrease with increasing atomic number (except for YZ03), i.e. La,O,, Nd,O, > Sm,O, > Eu,O, > Gd,O, > Dy,O, , suggesting that the mobilities of lattice
25 C* Selectivity
Fig. 1. Effect of time on stream over (a) SrF,/La,O, (1:4) at 7OO”C, (b) SrF,/Nd,O-, the conditions of CH,:O, = 3:l (no dilution gas) and GHSV = 20000 h-l_
C2 Yield (‘9%)
Time @) (1:l) at 75O”C, (c) SrF/Y,O,
(2:l) at 750°C under
R. Long et al. / Catalysis Today 30 (1996) 59-65
oxygen may also decrease in this order. For those rare earth oxides with higher mobility of lattice oxygen, the anionic exchange between oxides and fluoride might be easier, which will be favorable to promote the interaction between the oxide and fluoride phases. From the data in Table 1, it is interesting to see that the decrease in C, yields of SrF,/Ln,O, catalysts follows the same order as the decrease in the conductivities of rare earth sesquioxides. In the next section, more discussion concerned with ionic exchange between rare earth sesquioxides and SrF, will be presented. As can be seen from Table 1, on both promoted and unpromoted REO catalysts, oxygen was almost completely consumed ( 2 95%) in the reactions carried out at 750°C or higher, which suggested that the results showed in Table 1 were obtained under an oxygenlimited condition. The stability of the catalytic performance of the SrF, promoted Ln,O, catalysts varied with the rare earth elements. The results in Fig. 1 shows the catalytic performance of three SrF,
promoted catalysts with respect to time on stream. The SrF,/La,O, (1:4) catalyst was characterized by a little increase in CH, conversion and decrease in C, selectivity at the early period of reaction, as a result, the C, yield remained almost constant within a period of 36 h on stream. However, CH, conversion and C, selectivity over SrFJNd,O, (1:l) catalyst gradually decreased over a period of 30 h on stream, leading to the decrease of C, yield from 19.6% to 15.2%. After that, both CH, conversion and C, selectivity remained almost unchanged in the following 15 h. The decrease of catalytic performance was also observed over the SrF,/Y,O, (2:l) catalyst during a period of 31 h on stream. The loss of F- from the catalysts as HF during the reactions appears not to be the only reason for the decrease in catalytic performance of the catalysts, because there is no a corresponding relation between the relative loss amounts of F- from catalysts and the variations of catalytic performances. 3.2. Structure characterization
1 . tetmgonal NdOF Arhombohedml NdOF x wthorhombic SICO:
Fig. 2. ZX-ray powder patterns of (a) Nd,O,, (b) fresh SrF, /Nd,O, (l:l), (c) used SrF, /Nd,O, (l:l), (d) SrF, samples.
The XRD measurements indicated that new phases such as tetragonal and rhombohedral NdOF were formed in the fresh SrF,/Nd,O, sample (Fig. 2), suggesting that, during the process of the catalyst preparation, part of the F- (r = 1.33 A> in SrF, and O*- (r = 1.32 A) in Nd,O, were substituted by O*- and F-, respectively. Partial ionic exchange between SrF, and La,O, phases and formation of the lanthanum oxyfluorides, such as tetragonal LaOF, may also happen in SrF,/La,O, system. Unfortunately, the diffraction lines of tetragonal LaOF [d = 3.35(100), 2.90(25), 2.06(60), 2.05(33), 1.76(22) and 1.75(44)] were overlapped with the characteristic diffraction lines of SrF, [d = 3.352(100), 2.900(25), 2.0508(80), 1.7486(52)] which made it difficult to identify the LaOF phase from a SrF,/La,O, catalyst. However, the formation of rhombohedral LaOF and LaF, have been detected by XRD in a similar lO%BaF,/La,O, catalyst . For the
R. Long et al. / Catalysis Today 30 (1996159-65 Table 2 The results of XRD analysis of the fresh SrF, /Ln,O, Composition
Catalyst SrF, /La,O, SrF, /La*O, SrF, /Sm,O, SrF, SrF, SrF, SrF,
(1:4) (1: 1) (1:l)
and structure a
cubic SrF,(w); hexagonal La,O,(s) cubic SrF,(s); hexagonal La,O,(vs) cubic SmzO, (vs); cubic SrF,(s); monoclinic Sm,O,(s) cubic Eu,O~(S); cubic SrF,(m) cubic Gd,O,(s); cubic SrFs(m) cubic Dy,O,(s); cubic SrF,(m) cubic Y,Os(vs); cubic SrF,(s)
/Eu,O, (1:l) /Gd,O, (1:l) /Dy,O, (1:l) /Y203 (2:l)
a vs -
very strong, s -
strong, m -
medium, w -
other samples, XRD only detected cubic SrF, and rare earth sesquioxide phases, such as hexagonal La,O,, cubic and monoclinic Sm,O,, cubic Eu,O,, cubic Gd,O,, cubic Dy,O,, and cubic Y203 (Table 2). Another interesting result from Table 2 was that the content of cubic Sm,O, in the SrF,/Sm,O, (1:2) catalyst was a little more than that of monoclinic phase, while the pure Sm,O, contained almost equal amounts of both phases, suggesting that cubic SrF, may play a certain role in stabilizing the cubic Sm,O, at high temperature. When the SrF,/Ln,O, catalysts were exposed to CH,/O, (3:l) at 750°C for about 1.5 h, orthorhombic SrCO, resulting from the reaction between SrO and CO, (by-product of MOC reaction) was detected in the SrF,/Nd,O, (1:l) (Fig. 2) and SrF,/La,O, (1:4) catalysts (Table 3). This result provides further experimental evidence for the anionic or cationic exchanges between SrF, and the Ln,O, phases. Besides, Table 3 The results of XRD analysis of the SrF, /Ln,O, reacting about 1.5 h at 750°C Catalyst
SrF, /Eu,O, SrF, /Y,O,
a vs -
and structure a
cubic SrF, (w); hexagonal La,O, orthorhombic SrCO, (w) cubic Sm,O, (s); cubic SrF,(s); monoclinic Sm,O, (vs); rhombohedral SmOF(w) cubic Eu,O, (s); cubic SrF, (m) cubic Y203 (vs); cubic SrF, (s); rhombohedral YOF (w)
very strong, s -
strong, m -
medium, w -
XRD also detected the formation of rhombohedral SmOF and YOF phases in the used SrF,/Sm,O, (1:l) and SrF,/Y20, (2:l) catalysts, respectively (Table 31, which indicated that the exchange between F- and O*- was more favorable under the conditions of MOC reaction, and H,O generated in the reaction might play a certain role in promoting such exchange. These results were also in line with the observation that the NdOF content in a used SrF,/Nd,O, (1: 1) catalyst was higher than that in the fresh (Fig. 2). Based on these results, it is reasonable to suggest that the anionic exchange between oxide and fluoride phases also happened more or less in a fresh SrF,/Sm,O, (1:l) or SrF,/Y,O, (2:l) catalyst, but the content of SmOF or YOF is probably too low to be detected by XRD. No formation of new phase was detected in the used SrF,/Eu,O, (1:l) catalyst. It has been generally accepted that one of the essential conditions for a compound with stable cationic valency to be a good MOC catalyst is the presence and the mobility of the anionic vacancies in the lattice, so as to adsorb and activate 0, during the reaction . According to the literature, the structure of cubic Ln,O, compounds is closely similar to that of the fluorite but with l/4 intrinsic oxygen vacancies [ 171. The structure of hexagonal Ln,O, can be described by slabs of OLn, tetrahedrons linked by three of their edges and forming a complex group cation (LnO),“+ separated by ionic oxygens 0 *- . The monoclinic structure is very similar to hexagonal, but the tetrahedrons are distorted . ‘Genetic’ vacancies also exist in the hexagonal structure of Ln,O, and monoclinic structure of Sm,O,. However, their concentrations are lower (ca. 17% of vacant positions in the oxygen sublattice) than those of cubic phase [181. The tetragonal NdOF can be expressed by the formula LnO,F,_,, (0.7
R. Long et al./ Catalysis Today 30 (1996) 59-6.5
rides are found to be of a single phase, which chemical composition is sharply defined and corresponds exactly to LnOF . This structure is also a slightly distorted CaF,-type structure. Taking into consideration the fact that many compounds with fluorite-type structure, such as alkaline earth halides, ZrO,, etc. have anion Frenkel defects and anionic vacancies , it is reasonable to postulate that the similar anionic vacancies might also exist in the oxyfluoride compounds with fluorite-like structure. On the other hand, the ionic exchange between the oxide and fluoride phases of a SrF,/Ln,O, catalyst may also lead to the formation of anionic vacancies and other lattice defects such as F-center or O- species in order to maintain electroneutrality. The presence of anionic vacancies and F-center in the above catalyst will be favorable to the adsorption and activation of 0, under the reaction condition.
4. Conclusions Based on the above results, it can be concluded that the extent of F- and 02- exchange in the SrF,/Ln,O, catalysts are in the order Nd, La > Sm, Y > Gd, Eu, Dy. For those rare earth oxides with higher mobility of lattice oxygen, the interaction between oxides and fluoride will take place easily, which will be favorable to the formation of new oxyfluoride compounds and lattice defects including anionic vacancies, F-centers and O- in the catalysts. The existence of anionic vacancies and the possible formation of F-centers of the oxyfluoride compounds will be favorable to the adsorption and activation of molecular oxygen under the MOC condition. The adsorption and activation of oxygen on the catalyst surface have been supported by the in situ FTIR spectroscopic observation of 0, adspecies with characteristic vibration frequency on the O,-adsorbed near 1113 cm-’ SrF,/Nd,O, (1: 1) and SrF,/La,O, (1:4) catalysts at 700°C and 650°C respectively [13,22]. On the other hand, the dispersion of F- on the
surface of the catalysts will also be helpful to the isolation of the surface ‘active oxygen’ centers and the improvement of the C, selectivity. Therefore, the highest C, yield was obtained over SrF, promoted Nd,O, and La,O, catalysts among these catalysts, whereas, due to the weak interaction between SrF, and Dy,O,, the promoting effect of SrF, was not apparent for MOC reaction over SrF,/Dy,O, (1: 1) catalyst.
Acknowledgements This work has been supported by the National Natural Science Foundation of China.
References [l] K. Otsuka, K. Jinno and A. Morikawa, Chem. Lett., (1985) 499.  K.D. Campbell, H. Zhang and J.H. Lunsford, J. Phys. Chem., 92 (1988) 750.  J.H. Lunsford, Catal. Today, 6 (1990) 3.  S. Lacombe, C. Geantet and C. Mirodatos, J. Catal., 151 (1994) 439.  2. Kalenik and E.E. Wolf, in A. Holmen et al. (Eds.), Natural Gas Conversion, Elsevier, Amsterdam, 1991, p. 97.  H. Yamashita, Y. Machida and A. Tomita, Appl. Catal. A: Gem, 79 (1991) 203.  A.Z. Khan and E. Ruckenstein, J. Catal., 138 (1992) 322.  R. Burch, G.D. Squire and SC. Tsang, Appl. Catal., 48 (1988) 105. t91 J.H. Lunsford, P.G. Hinson, M.P. Rosynek, C. Shi, M. Xu and X. Yang, J. Catal., 147 (1994) 301. [lOI D. Wang, M.P. Rosynek and J.H. Lunsford, J. Catal., 151 (1995) 155. Dll X.P. Zhou, W.D. Zhang, H.L. Wan and K.R. Tsai, Catal. Lett., 21 (1993) 113. ml X.P. Zhou, S.Q. Zhou, S.J. Wang, J.X. Cai, W.Z. Weng, H.L. Wan and K.R. Tsai, Chem. Res. Chin. Univ., 9(3) (1993) 264. [131 X.P. Zhou, S.Q. Zhou, W.D. Zhang, Z.S. Chao, W.Z. Weng, R.Q. Long, D.L.Tang, H.Y. Wang, S.J. Wang, J.X. Cai, H.L. Wan and K.R. Tsai, Preprints, Division of Petroleum Chemistry, Vol. 39(2), ACS, 1994, p. 222. [141 K.A. Gschneidner, Jr. and L. Eyring, Handbook on the Physics and Chemistry of Rare Earth, Vol. 3, North-Holland, 1979, Chap. 27, p. 385. D51 CT. Au, H. He, S.Y. Lai and CF. Ng, Proc. 1st Global Conf. Young Chinese Scientists on Catalysis Science and Technology, Tianjin, China, 12-15 Sept. 1995, p. 193. [161A.G. Anshits, E.N. Voskresenskaya and L.I. Kurteeva, Catal. Lett., 6 (1990) 67.
R. Long et al. / Catalysis Today 30 (1996) 59-65  K.A. Gschneidner, Jr. and L. Eyring, Handbook on the Physics and Chemistry of Rare Earths, Vol. 5, North-Holland, 1982, Chap. 44, p. 322. 1181 E.N. Voskresenskaya, V.G. Roguleva and A.G. Anshits, Catal. Rev.-Sci. Eng., 37(l) (1995) 101.  K. Niihara and S. Yajima, Bull. Chem. Sot. Jpn., 44 (1971) 643.
 A. F. Wells, Structural Inorganic Chemistry, 5th edn., Oxford Univ. Press, NY, p. 483.  Z. Zhang, M. Baems et al., Catal. Rev.&i. Eng, 36(3) (1994) 507. 1221 R.Q. Long, H.L. Wan, H.L. Lai and K.R. Tsai, Chem. J. Chin. Univ., in press.